reaction. highly active and methanol-tolerant ... azhar mahmood, nanhong xie, muhammad aizaz ud din,
Post on 22-Jul-2020
Embed Size (px)
Electronic Supplementary Material (ESI) for Chemical Science.
Shape Controlled synthesis of porous tetrametallic PtAgBiCo nanoplates as highly active and methanol-tolerant electrocatalyst for Oxygen Reduction Reaction. Azhar Mahmood, Nanhong Xie, Muhammad Aizaz Ud Din, Faisal Saleem, Haifeng Lin, Xun Wang*
Key Lab of Organic Optoelectronics and Molecular Engineering, Department of Chemistry, Tsinghua University, Beijing 100084, China. E-mail: email@example.com
Pt(acac)2, AgNO3, Cu(acac)2, Fe(acac)2, Pd(acac)2, RhCl3, Co(acac)2 poly(vinylpyrrolidone) (PVP; Mw 8000), were purchased from Alfa Aesar Co.Ltd, and Bi(NO3)2, KI, KBr, KCl, tris (hydroxymethyl ) aminomethane, HCHO solution (37 wt%), formamide, and acetone were purchased from Sinopharm Chemical Reagent Co. Ltd . All the chemicals were analytical grade and used as received without any purification for the Synthesis of PtAgBi, PtAgBiCo nanoplates and PtAg, PtBi, PtCo, PdAgBi, RhAgBi nanostructures.
Synthesis of PtAgBi Nanoplates: PtAgBi NPLs synthesis were carried out by two-step method. In the first step a mixture of 50 mg tris and 200 mg PVP was dissolved in 2 mL HCHO solution and transferred to Teflon-lined stainless steel autoclave which was heated at 200°C for 3 hours. A gel like material was obtained, after the washing and centrifugation in acetone. Then in the second step a homogeneous solution of 0.01mmol Pt(acac)2, 0.01mmol AgNO3, 0.01mmol BiNO3, and 0.06 g KI was prepared in 2 ml formamide solvent and pour into 12 ml Teflon-lined stainless steel autoclave along with gel like material which was prepared in the first step, and kept the autoclave in oven at 140°C for 3 h. Final product was obtained after washing by using acetone. Synthesis of PtAgBiCo Nanoplates: The synthesis procedure and experimental conditions for PtAgBiCo nanoplates were same as the PtAgBi nanoplates, except that, we added Co(acac)2 precursor in the second step for tetrametallic nanoplates and the reaction time was increased from three hours to six hours. Synthesis of PdAgBi and RhAgBi Nanostructures: The synthesis procedure and experimental conditions for PdAgBi and RhAgBi nanostructures were same as the PtAgBi nanoplates, except that, we replaced Pt(acac)2 by Pd(acac)2 for the synthesis of PdAgBi nanostructures and for RhAgBi nanostructures we replaced Pt(acac)2 by RhCl3 respectively. Synthesis of PtAg, PtBi, PtCo Nanostructures: For PtAg nanostructures, synthesis were carried out by two-step method. Firstly, a mixture of 50 mg tris and 200 mg PVP was dissolved in 2 mL HCHO solution and transferred to Teflon-lined stainless steel autoclave which was heated at 200°C for 3 hours. A gel like material was obtained, after the washing and centrifugation in acetone. Secondly, a homogeneous solution of 0.01mmol Pt(acac)2, 0.01mmol AgNO3, and 0.06 g KI was prepared in 2 ml formamide solvent and pour into 12 ml Teflon-lined stainless steel autoclave along with gel like material which was prepared in the first step, and kept the autoclave in oven at 140°C for 3 h. Final product was obtained after washing by using acetone. Similarly, PtBi and PtCo nanostructures were synthesized, for
Electronic Supplementary Material (ESI) for Chemical Science. This journal is © The Royal Society of Chemistry 2017
PtBi all the reaction conditions were similar as PtAg except we replace AgNO3 by BiNO3, and for PtCo nanostructures synthesis we added Co(acac)2 along with Pt(acac)2 . Electrochemical Measurements:
Oxidation reduction reaction (ORR) electrochemical measurements of PtAgBi and PtAgBiCo catalyst were performed using a standard RDE system. Electrochemical test was performed on Princeton P4000 electrochemical workstation, using three electrode cell. The reported potentials are specified relative to the RHE scale. Prior to the experiment, glassy electrode was polished with alumina suspensions powder to yield a mirror finish on a felt polishing pad. Then, as prepared PtAgBi, PtAgBiCo nanoplates or Pt/C NPs were dispersed in 0.80 mL of H2O, 0.20 mL of ethanol, and 10 µL of Nafion solution (0.05 wt%) by soniocation for more than 1 h to form a homogeneous catalyst ink. The catalyst ink was transferred to the surface of the glassy carbon (GC) electrode and dried at room temperature. ORR measurements were performed oxygen saturated 0.1 M HClO4 solutions using GC-RDE at a scan rate of 10 mV s−1 with or without methanol at a rotation speed of 1600 rpm and CV measurements were performed in N2- saturated solutions. The mass activity, which is the current per unit mass (molar conc. determined through ICP-OES analysis) of the Pt/C and PtAgBiCo/C Catalyst, is the corresponding current at the potential of 0.9 V RHE and mass of samples can be calculated. For CO-stripping experiment to calculate ECSA, the catalyst was saturated with high purity CO by bubbling CO into the electrolyte for 25 min. By flowing N2-gas for 15 min, the residual CO was then removed. The CO-stripping curve was recorded from 0.05 to 1.55 V with a scanning rate of 50 mV s−1. The CO-ECSA value was calculated by integration of charges between 0.82 and 1.1 V using the charge between the first and second cycles. The measured charge was then normalized using the theoretical value of 420 µC cm−2, mass of catalystPt, and scanning rate, i.e., 50 mV s−1. In CV curve the current densities were normalized reference to the geometric area of RDE(0.196cm2). Characterization: Transmission electron Microscopy (TEM) and high-resolution transmission electron microscope (HRTEM) were recorded on a HITACHI H-7700 TEM with an accelerating voltage of 100 kV, and FEI Tecnai G2 F20 S-Twin high-resolution TEM equipped with energy dispersive spectrometer (EDS) analyses at 200 Kv. The samples for HRTEM analysis were prepared by dropping ethanol dispersion of samples onto 300-mesh molybdenum grids. X-ray diffraction (XRD): XRD patterns were measured with a Bruker D8-advance X-ray powder diffractometer operated at 40 KV voltage and instrument run at a scan rate of 0.02 deg / s in the angle range of 5° to 90° and the wave length of the incident radiation was λ = 1.5418 Å. X-ray photoelectron spectroscopy (XPS): XPS measurements were conducted on a scanning X-ray microprobe (Quantera SXM, ULVAC-PHI. INC) operated at 250 kV, 55 eV with monochromated Al Kα radiation. ICP-OES: Elemental analysis of the samples was determined by inductively coupled plasma atomic emission spectrometry (ICP-AES, IRIS Intrepid Ⅱ XSP, Thermo Fisher).
Acknowledgements This work was supported by NSFC (21431003, 21521091) and China Ministry of Science and Technology under Contract of 2016YFA0202801.
Figure S1. HRTEM image of triangular PtAgBiCo nanoplates.
Figure S2. HRTEM image of PtAgBi nanoplates.
Figure S3. HRTEM image of hexagonal PtAgBi nanoplates.
Figure S4. HRTEM image of triangular PtAgBi nanoplates.
Figure S5. XRD patterns of (a) PtAgBi 1 and (b,c) PtAgBiCo 2 Nanoplates, where b) and c) are with 0.005 and 0.01 molar concentration of cobalt.
The XRD patterns shows that there are no diffraction peaks of the individual metal Pt, Ag, Bi or Co that would indicate the formation of single-phase alloys. In the PtAgBi alloy, all of the diffraction peaks are shifted to higher angles toward Bi Fig.S5a (Pt1Bi1-ICSD#58545) compared with the standard diffraction patterns for pure Pt (Pt-JCPDS no.04-0802) and Ag (Ag-JCPDS no.04-0783) references. While after addition of cobalt with low concentration, the diffraction peaks of the alloy start to shift toward Pt and Co (Co-JCPDS no.150806) references Fig.S5b. This slight shifting of the peaks after addition of low concentration of cobalt is the indication of the incorporation of cobalt and the formation of the tetrametallic PtAgBiCo alloy. Meanwhile, after the addition of an appropriate concentration of the cobalt, where we obtained tetrametallic PtAgBiCo nanoplates with only one kind of morphology (Triangular), the corresponding diffraction peaks of PtAgBiCo alloy more shifted toward Pt and Co references Fig.S5c. It is indicating that the introduction of Co, generates tetrametallic NPLs with only one kind of morphology (Triangular).
Figure S6. TEM images of nanoplates prepared with different molar ratios of Pt(acac)2, AgNO3, Bi(NO3)2, and Co(acac)2: a) 0.01:0.01:0.01, b) 0.01:0.01:0.01 and 0.005 c) 0.01:0.01:0.01 and 0.01 d) 0.01:0.01:0.01 and 0.015.
Figure S7. a) STEM-HAADF b) line-scanning profile and c) HRTEM images of PtAgBi Twin nanoparticles ST= single twin and DT= double Twin.
Figure S8. TEM images of as prepared PtAgBi a) reentrant groves and b) its transformation into hexagonal and triangular nanoplates.
Figure S9. TEM images of as prepared PtAgBi nanostructures at a) 5 min, b) 20 min, c) 40 min, d) 60 min, e) 120 min, f) 180 min and g) 360 minutes reaction time.
Figure S10. TEM images of as prepared PtAgBiCo nanostructures at a) 5 min, b) 60 min, c) 120 min, d) 180 min, e) 360 minutes reaction time.
Figure S11. Schematic illustration of multimetallic nanoplates.
Figure S12. TEM images of as prepared a) PtAgBiFe and b) PtAgBiCu nanostructures at 180 minutes reaction time.
Figure S13. TEM images of as prepared a) PtAgBi nanoplates at 180 min and b) PtAgBiCo nanoplates at 360 minutes reaction time after Purged with Ar gas.
Figure S14. TEM images of the PtAgBi products collected after three hour reactions time where different halide